Research Article  Open Access
Milena Rangelov, Somayeh Nassiri, "Evaluation of Methods to Correct the Effect of Temperature on Electrical Conductivity of Mortar", Advances in Civil Engineering, vol. 2018, Article ID 9327528, 9 pages, 2018. https://doi.org/10.1155/2018/9327528
Evaluation of Methods to Correct the Effect of Temperature on Electrical Conductivity of Mortar
Abstract
Nondestructive methods to obtain the electrical conductivity (σ) or resistivity (ρ) of concrete are gaining popularity for durability evaluation. However, these methods are susceptible to the effects of curing and conditioning, primarily temperature and degree of saturation. Before σ of concrete at varied temperatures can be used for durability assessment, appropriate corrections must be made to account for the effect of temperature (T). In this study, two existing and one new temperature correction methods were evaluated for 12 mortar mixtures varying in watertocementitious material ratio (w/cm) and the content and types of supplementary cementitious materials (SCM). Mortar specimens instrumented with embedded sensors were cured in sealed conditions for 11–13 months. After this period, the sealed specimens were subjected to stepwise temperature change in 5–50°C range while σ was recorded using the embedded sensors. Linear, bilinear, and Arrhenius temperature correction (LTC, BLTC, and ATC, respectively) were fitted to the obtained σT datasets and were evaluated for fitness. LTC provided an acceptable fit to the σT data (R^{2} > 0.81) but was found the most suitable in 5–30°C temperature range. BLTC was defined as a combination of two distinct LTC below and above the reference temperature at 23°C and had a better fit to the data (R^{2} > 0.96). Lastly, ATC showed the best fit among the tested methods (R^{2} > 0.98) and was found applicable for the full tested temperature range. Comparison of correction coefficients among the mixtures indicated that increase in w/cm results in less sensitivity of σ to temperature. Mixtures with SCM generally exhibit higher temperature sensitivity compared to the corresponding plain mixture. Since the variations in correction coefficients were not substantial (less 18% variation among 10 of 12 mixtures), a single value of activation energy of conduction (E_{c}) at 32 kJ/mol was identified as the general recommendation for all the tested mixtures.
1. Introduction
In recent years, nondestructive techniques for indirect assessment of concrete transport properties and durability by measuring electrical conductivity (σ) or resistivity (ρ) have gained popularity [1]. The measurements are taken by several available methods based on uniaxial or bulk resistivity, surface resistivity, electrical impedance spectroscopy, and noncontact resistivity measurements based on the transformer principle [1–5]. Additionally, embedded sensors for realtime ρ monitoring were evaluated in past studies [6–8]. Since electrical current in the concrete is primarily conducted through the pore solution in the pore system, electrical measurements can be used to indirectly evaluate pore system and transport properties of concrete [5, 6, 9, 10]. Relatively high ρ (low σ) is a characteristic of concrete with dense microstructure, low porosity, and poorly interconnected pores. This type of microstructure hinders the ingress of water and ions that typically leads to durabilityrelated distresses. In several research studies, σ or ρ were utilized to evaluate chloride diffusivity or permeability, which is a key input for service life predictions of reinforced concrete structures exposed to chlorides [7,11–13]. Due to simplicity, rapid nature, and nondestructive nature of the data collection, as well as availability of commercial apparatus, electrical methods are becoming more common in concrete durability evaluation [14, 15].
Despite the convenience of these methods, data interpretation still requires more research as multiple factors, such as mixture design, temperature, and degree of saturation, have combined influences on the results [1, 16]. The synergistic effect of these factors should be taken into consideration when interpreting σ or ρ data in cementitious systems. The focus of this study is the effect of temperature and evaluation of existing correction methods.
Changes in temperature (T) induce changes in the ionic mobility, pore solution concentration, and iontoion and iontosolids interactions in the pore solution, which result in changes in the overall conductivity of the concrete [14]. Since accurate assessment of these effects is complex and difficult, the effect of temperature on σ is typically evaluated empirically. The simplest type of σT dependency investigated in the literature is linear, typically defined through linear temperature correction (LTC) [8,17–19]:where is the reference temperature in °C, typically defined in a value in the 21–25°C range, and are the resistivity and conductivity at , is the conditioning temperature in °C, and α is a linear correction coefficient (%/°C). The recommended values of α range from 3 to 5% per 1°C temperature increase [17–19]. However, LTC was found effective only in a small temperature range (±5°C of the reference temperature) [20].
In addition to LTC, the Arrhenius form equation was used in the literature for temperature correction (hereafter: ATC) [3, 8, 16, 17, 20, 21]:where is the universal gas constant (8.314 J/molK) and is the activation energy of conduction in kJ/mol. Higher values of correction coefficients ( and for LTC and ATC, respectively) indicate higher temperature sensitivity of the mixture [17]. Typical values of from the literature range from 12.54 to 42.47 kJ/mol and primarily depend on the degree of saturation, with sealed specimens presenting higher compared to the saturated ones [3, 8, 16, 17, 20, 21].
Spragg et al. compared temperature correction of ρ for saturated concrete specimens measured by the uniaxial versus the surface resistivity method and found that surface resistivity method yields E_{c} that are 7 to 15% higher than that by the uniaxial method [16]. The identified difference in E_{c} was attributed to the effects of leaching occurring on the surface of the specimen detected by surface resistivity meter [16]. Weiss et al. evaluated the LTC and ATC methods for 13 concrete mixtures varying in watertocementitious materials ratio (w/cm) and binder type (Portland cement, binary, and ternary mixtures) for 5 < T_{c} < 30°C by uniaxial resistivity method [17]. Saturated specimens were found to be less sensitive to temperature (smaller values of α and E_{c}) compared to their sealed counterparts, and both LTC and ATC were found satisfactory. However, due to higher temperature sensitivity of the sealed specimens, ATC was recommended as the reliable temperature correction method [17].
As reviewed above, the effectiveness of various temperature correction methods was evaluated in only one study. The suitability of current methods at higher temperatures (30–50°C) which is representative of inservice conditions in hot climate areas is yet to be evaluated. Further, the effect of mixture parameters and SCMs on temperature sensitivity of mixes requires more investigation. The effectiveness of the correction methods for data collection methods other than uniaxial resistivity method deserves further research. Currently, the electrical characterization methods are mostly limited to laboratory conditions, whereas the appropriate durability characterization would require realtime in situ durability assessment. This can be achieved by the use of embedded electrical sensors; however, appropriate corrections for environmental conditions have to be applied. So, this study puts forward a framework for temperature corrections of sensorbased σ, which is a necessary step for in situ durability evaluation.
In this study, sensorbased σ data are used from a variety of mortar mixtures over a wide temperature range from 5 to 50°C to investigate the effectiveness of both the LTC and ATC methods. Temperature sensitivity of mixes containing varied w/cm and contents of ground granulated blast furnace slag (GGBFS), class F fly ash, and silica fume is investigated. Recommended values for the correction parameters of each method are developed based on the tested mixtures.
2. Description of Experiment
2.1. Materials and Mixtures
The experimental matrix included 12 mortar mixture designs with proportioning listed in Table 1. Implemented aggregate was river sand with specific gravity 2.51 and fineness modulus 3.06. A reference mixture (control) was prepared with ordinary type I/II Portland cement, w/cm of 0.45, and aggregatetobinder ratio of 1.95. The remaining 11 test mixtures had the same aggregatetobinder ratio as the control but varied in water content and cementitious materials as follows:(i)W mixtures with varied w/cm at 0.35, 0.40, and 0.50(ii)GGBFS mixtures with partial cement replacement by GGBFS at 20 and 40 percent by mass (GGBFS_20, GGBFS_40)(iii)Fly_ash mixtures with partial cement replacement by class F fly ash at 20, 40, and 60 percent by mass (Fly_ash_20, Fly_ash_40, Fly_ash_60)(iv)S_fume mixtures with partial cement replacement by class silica fume at 5, 10, and 15 percent by mass (S_fume_5, S_fume_10, S_fume_15)

Chemical composition of cementitious materials used in the study is provided in Table 2.
 
Fineness of fly ash was 26.6 percent of retained on 45 μm (no. 325) standard sieve. Blaine fineness was not available. 
2.2. Specimen Casting and Instrumentation
Mortar mixtures specified in Table 1 were prepared following ASTM C305 [22]. One Φ100 by 200 mm cylindrical specimen per mixture was cast and kept in sealed conditions in a plastic mold for electrical conductivity measurements. Electrical conductivity was measured using one embedded timedomain reflectometry (TDR) sensor, Type 5TE from Meter Group [23]. The 5TE sensor was used to measure T and electrical conductivity (σ) of the mortar. The sensor applies an electrical current to and measures the resistivity of the medium between the sensor probes. This type of sensor is currently used in soil applications for the assessment of soil salinity and water content. The authors demonstrated the application of the sensors in cementbased materials in earlier publications [6, 7]. In this study, one 5TE sensor was vertically embedded at middepth location of each cylinder specimen during casting. All sensors were connected to a CR1000 datalogger from Campbell Scientific, and the sensor data were recorded in 5minute intervals. Specimens were covered at the top with double plastic bags during the first 24 hours. After this initial period, while the specimens were kept in their molds, the plastic bags were removed, and the tops were sealed using adhesive aluminum tape. Specimens were kept in the sealed condition in the laboratory with controlled ambient temperature at 21°C for 11–13 months.
2.3. Temperature Regimes
The specimens were placed in a temperaturecontrolled chamber and were subjected to stepwise temperature change, T_{c}’s: 5, 10, 15, 23, 30, 40, and 50°C. Each T_{c} was kept constant for approximately five days until the sensorbased measurements of T and σ exhibited minimal fluctuations (standard deviation of T < 0.1°C and standard deviation of σ < 0.005 dS/m). The temperature regime based on the sensor in mix W0.35 is provided in Figure 1 as an example.
3. Results and Data Analysis
3.1. Effect of Temperature on Electrical Conductivity of Mix Groups
Figure 2 presents the changes in σ as a function of T for all the tested mixtures. Each data point is the average of all of σ and T data during one T_{c} step. As seen in Figure 2, σ increases as temperature is increased for all the tested mixtures. This trend is expected, since the increase in T is associated with increased mobility of ions in the pore solution, resulting in higher conductivity [14]. At T_{c} > 23°C, σ increases at a faster rate with the same incremental increase in temperature (exponential Tσ trend.) Therefore, T_{c} = 23°C is used as the reference temperature in the following sections.
(a)
(b)
(c)
(d)
The effect of mixture parameters can be identified based on the difference in the values of σ among the different mixtures in Figure 2(a); mixtures with lower w/cm exhibit lower values of σ, as an effect of lower amount of pore solution in the pore system, as well as less connected (more tortuous) capillary pores [6, 24, 25]. In Figures 2(b)–2(d), the use of SCM results in overall lower values of σ compared to the plain mixture and the more use of SCM results in lower values of conductivity. The trend is due to the products of SCM late pozzolanic reaction, which fills the capillary pores, making the pore system discontinuous and less conductive [6, 26, 27]. At T_{c} < 23°C, σ data of GGBFS_40, Fly_ash_40, and Fly_ash_60 approach nearzero values. Since the accuracy of 5TE sensors is 0.01 dS/m, the absolute values of σ may not be reliable for these sensors.
3.2. Linear Temperature Correction (LTC)
Linear temperature correction (equation 1) was applied to the experimental Tσ data shown in Figure 3. The effective conductivity at T_{c} = 23°C is marked as σ_{ref}. Figure 3 presents the σ/σ_{ref} ratio at various T_{c} based on the experimental data and the fitted LTC for all the mixtures. The calibrated values of coefficient α were determined using the Solver function in Microsoft Excel, such that the sum of the squared differences between the measured and corrected σ/σ_{ref} is minimized. Table 3 shows the calibrated α values and high coefficients of determination (R^{2} > 0.81) for the fitted lines. However, for several mixtures, LTC results in negative σ values for T_{c} = 5°C, which bears no physical meaning and should be assumed as zero. Also, the values of α obtained in this study are higher than those for concrete reported by Weiss et al., ranging from 1.87–3.37%/°C [17]. The temperature range in [17] was 5–30°C, compared to 5–50°C in this study. The higher T_{c}, results in a steeper exponential σT correlation, therefore LTC produces suboptimal fit to the data. The temperature range of 5–30°C seems to be the optimum range for the LTC model. To address this limitation, different temperature corrections are evaluated in Sections 3.3. and 3.4.
(a)
(b)
(c)
(d)

3.3. New Bilinear Temperature Correction (BLTC)
Based on the results in Figure 3, the rate of change in σ with T_{c} is different above and below the reference temperature. Therefore, a bilinear temperature correction (BLTC) model is proposed here, with two individual temperature coefficients (α_{1} and α_{2}) for the ranges below and above T_{ref}:
Values of α_{1} and α_{2} for each mixture were determined using the Microsoft Excel Solver functions as described in Section 3.2. The calibrated coefficients α_{1} and α_{2}, with the corresponding R^{2} values for BLTC are listed in Table 4. The experimental data and the new model are plotted versus T_{c} in Figure 4. As seen in Table 4, the new model provides a better fit to the data compared to the LTC (Table 3) (R^{2} > 0.96.) The fitted values for the coefficients α_{2} are higher than the α_{1} values, indicating higher temperature sensitivity when T_{c} > T_{ref}. Calibrated values of α_{1} are within the range identified by Weiss et al.; however, values of α_{2} surpass the 1.87–3.37%/°C range due to higher T_{c} used in this study [17]. With a better fit to the data, the new BLTC model presents a promising alternative to LTC for a wide range of temperature.

(a)
(b)
(c)
(d)
3.4. Arrhenius Temperature Correction (ATC)
Temperature correction based on E_{c}, defined earlier in equation 2 as ATC, was applied to the experimental σT data. Optimal values of E_{c} for each mixture are provided in Table 5 with the corresponding R^{2}. Figure 5 presents the experimental σ/σ_{ref} data and the fitted ATC model for all mixtures. As seen in Table 5, ATC provides a better fit to the data compared to the LTC and BLTC methods (R^{2} > 0.98). The values of E_{c} fall in the 23.4 to 42.47 kJ/mol range, which is reported for sealed concrete in the literature [3, 8, 17].

(a)
(b)
(c)
(d)
3.5. Effect of Mixture Design on Temperature Sensitivity
The temperature sensitivity of σ measurements for each mixture can be inferred from the values of the correction coefficients (α and E_{c}), listed previously in Tables 3–5. Based on the obtained results, higher w/cm decreases the sensitivity of σ of the mix to temperature. This trend is consistent with findings of Weiss et al., who reported lower temperature sensitivity of specimens at higher degree of saturation [17]. It is possible that the diluted pore solution of mixtures with higher w/cm exhibits less increase in ionic mobility at elevated temperatures. Mixtures with SCM generally exhibit higher sensitivity to temperature correction compared to the control mix; the only exceptions are S_fume_5 and S_fume_10. It is likely that the differences in temperature sensitivity are due to the differences in pore solution alkalinity and chemical composition. It is also noteworthy that Fly_ash_60 and GGBFS_40 have the highest values of E_{c} due to low σ at T_{c} = 5°C. The value of σ at this low temperature is close to the sensor’s limit of sensitivity so if the two mixtures are removed from the data, the values of E_{c} are within a relatively narrow range for all mixtures (maximum difference among E_{c} values is 18%). It is therefore beneficial to determine a single average value of E_{c} for all mixtures as shown in Figure 6. The calibrated value of E_{c} is 32 kJ/mol, and the fit is satisfactory (R^{2} = 0.97).
4. Conclusions
An experimental study was conducted with the primary objective to evaluate existing temperature correction methods for electrical conductivity (σ) of concrete. Twelve mortar mixtures were kept in stepwise temperature change in 5–50°C range. Three methods of linear, bilinear, and Arrhenius temperature correction (LTC, BLTC, and ATC) were evaluated. Results revealed that LTC gives acceptable fit to the experimental data only for the temperatures up to 30°C. Bilinear temperature correction, with different coefficients below and above the reference temperature of 23°C, presented a favorable alternative to linear correction. Lastly, ATC provided the best fit among all methods over the full temperature range. Comparison of different mixtures indicated that increase in watertocementitious ratio yields lower temperature sensitivity. The implementation of supplementary cementitious materials generally increased the responsiveness of σ to the temperature change. As the values of temperature correction coefficients did not vary substantially among the tested mixtures, a single E_{c} at 32 kJ/mol is recommended for all tested mixtures. Future research will include a wider range of mixture designs and evaluation of the established corrections for different electrical methods, such as axial and surface resistivity meters.
Data Availability
The temperatureconductivity data used to support the findings of this study are available from the corresponding author upon request.
Conflicts of Interest
The authors declare that there are no conflicts of interest.
Acknowledgments
Funding was provided by Portland Cement Association fellowship award. The authors acknowledge Meter Group for providing the instrumentation and technical support for this study. Premix Pullman is acknowledged for aggregate donation. Thanks to Ash Grove Cement Company for supplying cement, Lafarge for fly ash and slag, and BASF for silica fume.
References
 H. Layssi, P. Ghods, A. R. Alizadeh, and M. Salehi, “Electrical resistivity of concrete,” Concrete International, vol. 37, no. 5, pp. 41–46, 2015. View at: Google Scholar
 L. Xiao and Z. Li, “Earlyage hydration of fresh concrete monitored by noncontact electrical resistivity measurement,” Cement and Concrete Research, vol. 38, no. 3, pp. 312–319, 2008. View at: Publisher Site  Google Scholar
 R. Spragg, C. Villani, K. Snyder, D. Bentz, J. W. Bullard, and J. Weiss, “Factors that influence electrical resistivity measurements in cementitious systems,” Transportation Research Record: Journal of the Transportation Research Board, vol. 2342, no. 1, pp. 90–98, 2013. View at: Publisher Site  Google Scholar
 J. Chen, Z. Li, and X. Jin, “Critical features of microstructure development of earlyage cement paste revealed by noncontact electrical resistivity measurement,” Construction and Building Materials, vol. 154, pp. 1121–1129, 2017. View at: Publisher Site  Google Scholar
 K. B. Sanish, N. Neithalath, and M. Santhanam, “Monitoring the evolution of material structure in cement pastes and concretes using electrical property measurements,” Construction and Building Materials, vol. 49, pp. 288–297, 2013. View at: Publisher Site  Google Scholar
 M. Rangelov and S. Nassiri, “Empirical timedependent tortuosity relations for hydrating mortar mixtures based on modified Archie’s law,” Construction and Building Materials, vol. 171, pp. 825–838, 2018. View at: Publisher Site  Google Scholar
 M. Rangelov and S. Nassiri, “Sensorbased timedependent formation factor in prediction of chloride ingress in mortar,” Magazine of Concrete Research, pp. 1–38, 2018. View at: Publisher Site  Google Scholar
 Y. A. Villagrán Zaccardi, J. Fullea García, P. Huélamo, and Á. A. Di Maio, “Influence of temperature and humidity on Portland cement mortar resistivity monitored with inner sensors,” Materials and Corrosion, vol. 60, no. 4, pp. 294–299, 2009. View at: Publisher Site  Google Scholar
 Z. Liu, Y. Zhang, and Q. Jiang, “Continuous tracking of the relationship between resistivity and pore structure of cement pastes,” Construction and Building Materials, vol. 53, pp. 26–31, 2014. View at: Publisher Site  Google Scholar
 M. R. Nokken and R. D. Hooton, “Using pore parameters to estimate permeability or conductivity of concrete,” Materials and Structures, vol. 41, no. 1, pp. 1–16, 2007. View at: Publisher Site  Google Scholar
 T. D. Rupnow and P. J. Icenogle, “Surface resistivity measurements evaluated as alternative to rapid chloride permeability test for quality assurance and acceptance,” Transportation Research Record: Journal of the Transportation Research Board, vol. 2290, no. 1, pp. 30–37, 2012. View at: Publisher Site  Google Scholar
 W. J. Weiss, R. P. Spragg, O. B. Isgor, M. T. Ley, and T. Van Dam, “Toward performance specifications for concrete: linking resistivity, RCPT and diffusion predictions using the formation factor for use in specifications,” in High Tech Concrete: Where Technology and Engineering Meet, pp. 2057–2065, Springer, Cham, Switzerland, 2018. View at: Google Scholar
 P. J. Tumidajski and A. S. Schumacher, “On the relationship between the formation factor and propan2ol diffusivity in mortars,” Cement and Concrete Research, vol. 26, no. 9, pp. 1301–1306, 1996. View at: Publisher Site  Google Scholar
 P. Azarsa and R. Gupta, “Electrical resistivity of concrete for durability evaluation: a review,” Advances in Materials Science and Engineering, vol. 2017, Article ID 8453095, 30 pages, 2017. View at: Publisher Site  Google Scholar
 S. W. Tang, X. H. Cai, Z. He et al., “The review of pore structure evaluation in cementitious materials by electrical methods,” Construction and Building Materials, vol. 117, pp. 273–284, 2016. View at: Publisher Site  Google Scholar
 R. Spragg, C. Villani, and J. Weiss, “Electrical properties of cementitious systems: formation factor determination and the influence of conditioning procedures,” Advances in Civil Engineering Materials, vol. 5, no. 1, pp. 124–148, 2016. View at: Publisher Site  Google Scholar
 J. Weiss, A. Amirkhanian, P. Suraneni, R. Spragg, and A. Coyle, “Comparison of linear temperature corrections and activation energy temperature corrections for electrical resistivity measurements of concrete,” Advances in Civil Engineering Materials, vol. 7, no. 1, pp. 174–187, 2018. View at: Publisher Site  Google Scholar
 W. J. McCarter, T. M. Chrisp, G. Starrs, P. A. M. Basheer, and J. Blewett, “Field monitoring of electrical conductivity of coverzone concrete,” Cement and Concrete Composites, vol. 27, no. 78, pp. 809–817, 2005. View at: Publisher Site  Google Scholar
 R. B. Polder, “Test methods for on site measurement of resistivity of concrete  a RILEM TC154 technical recommendation,” Construction and Building Materials, vol. 15, no. 23, pp. 125–131, 2001. View at: Publisher Site  Google Scholar
 T. M. Chrisp, G. Starrs, W. J. McCarter, E. Rouchotas, and J. Blewett, “Temperatureconductivity relationships for concrete: an activation energy approach,” Journal of Materials Science Letters, vol. 20, no. 12, pp. 1085–1087, 2001. View at: Publisher Site  Google Scholar
 W. J. McCarter, “Effects of temperature on conduction and polarization in Portland cement mortar,” Journal of the American Ceramic Society, vol. 78, no. 2, pp. 411–415, 1995. View at: Publisher Site  Google Scholar
 ASTM C305/C30514, 2014, Standard Practice for Mechanical Mixing of Hydraulic Cement Pastes and Mortars of Plastic Consistency, ASTM International, West Conshohocken, PA, USA, 2014.
 Meter Group, ECH_{2}O 5TE Soil Moisture, Temperature, and Electrical Conductivity Sensor, 2018, https://www.metergroup.com/environment/products/ech2o5teelectricalconductivity/.
 J. Weiss, T. J. Barrett, C. Qiao, and H. Todak, “Toward a specification for transport properties of concrete based on the formation factor of a sealed specimen,” Advances in Civil Engineering Materials, vol. 5, no. 1, pp. 179–194, 2016. View at: Publisher Site  Google Scholar
 X. Chen and S. Wu, “Influence of watertocement ratio and curing period on pore structure of cement mortar,” Construction and Building Materials, vol. 38, pp. 804–812, 2013. View at: Publisher Site  Google Scholar
 B. Lothenbach, K. Scrivener, and R. D. Hooton, “Supplementary cementitious materials,” Cement and Concrete Research, vol. 41, no. 12, pp. 1244–1256, 2011. View at: Publisher Site  Google Scholar
 M. C. G. Juenger and R. Siddique, “Recent advances in understanding the role of supplementary cementitious materials in concrete,” Cement and Concrete Research, vol. 78, pp. 71–80, 2015. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2018 Milena Rangelov and Somayeh Nassiri. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.